**PAPER • OPEN ACCESS**

## Simulation of electron energy loss spectra with the turboEELS and

## thermo_pw codes

**To cite this article: Oleksandr Motornyi et al 2018 J. Phys.: Conf. Ser. 1136 012008**

View the article online for updates and enhancements.

## Simulation of electron energy loss spectra with the

## turboEELS and thermo pw codes

Oleksandr Motornyi1, Mich`ele Raynaud1, Andrea Dal Corso2,

Nathalie Vast1

1

Laboratoire des Solides Irradi´es, ´Ecole Polytechnique CEA DRF IRAMIS -CNRS UMR 7642, Paris-Saclay University, 91128 Palaiseau c´edex, France

2

Scuola Internazionale Superiore di Studi Avanzati (SISSA), Via Bonomea 265, IT-34136 Trieste, Italy, IOM-CNR Trieste, Italy

E-mail: oleksandr.motornyi@polytechnique.edu Abstract.

For some materials like noble metals, electron energy loss spectra have a complex structure that makes them difficult to analyze without the help of ab initio calculations. Various theoretical approaches can be used for this purpose, among which the time-dependent density functional perturbation theory (TDDFPT) which has been widely used to study plasmons in a number of bulk and surface systems. In the present paper we present a comparison of the results and performance of two different numerical implementations of TDDFPT: the Sternheimer and Liouville-Lanczos methods. The former approach is implemented in the thermo pw module and the latter one in the turboEELS code of the Quantum ESPRESSO package for electronic structure calculations. In the present paper a comparison is made for bulk bismuth, a semimetal, taking into account spin-orbit coupling, as well as for bulk gold, a noble metal. We show that for these two examples, both codes gives identical results and the turboEELS code has a better performance than the thermo pw code, and point out in which cases the usage of thermo pw alone or of both codes can be advantageous.

1. Introduction

Electron energy loss (EEL) spectroscopy [1] is a powerful experimental method that allows one to measure the change in kinetic energy -the energy loss- of electrons after their interaction with a sample. This technique can be used to obtain structural and chemical information about a specimen -from the high-energy loss region of the spectra- as well as information about valence electron excitations -from the low-energy loss region of the spectra-. In particular, the valence region of the spectra contains information about the band structure and dielectric properties of the material: plasmons, surface plasmons and interband transitions. For some materials like aluminum, valence EEL spectra has a simple structure containing one single, well-defined, plasmon peak for which the Drude model is a pertinent approximation. In materials where the behavior of valence electron is far from the (quasi) free electron model however, the EEL spectrum contains many peaks from single, to collective and to superposition of collective and single excitations, that make it difficult to analyze.

In order to perform a thorough analysis it is convenient to simulate EEL spectra computing the dielectric function. Indeed, in an EEL spectroscopy experiment, the inelastic scattering

2

probability of an incoming electron by the electrons of the solid, given by the double-differential cross-section d2σ/(dωdΩ) is measured, which is linked to the macroscopic dielectric function M:

d2σ

dωdΩ ∼ Im[

1 M(Q, ω)

], (1)

where Q is a momentum transfer, ω is an electron energy loss, and dΩ is the elemental solid-angle in which the scattering occurs.

Various ab initio methods that allow one to calculate spectral properties of solids have been developed in the past decades, addressing different aspects of the problem [2]. Time-dependent density functional theory (TDDFT) has been widely used to study plasmons in a number of bulk and surface systems [3, 4]. We note however that even for a material as simple as covalent silicon, one might need to account for many-body (excitonic) effects beyond TDDFT for instance to properly describe the shape of the plasmon peak [5].

In the present paper we will focus on the time-dependent density functional perturbation theory (TDDFPT) and linear response approach [6, 7] to the calculation of the dielectric

function. Two implementations, the Sternheimer and Liouville-Lanczos methods, will be

compared for bulk bismuth and gold. The paper is organized as follows. In Sec. 2, a

brief overview and comparison of the theoretical methods: classic TDDFT approach, and the Liouville-Lanczos and Sternheimer approaches to TDDFPT, will be given. In Sec. 3, results obtained using different approaches and corresponding implementations will be shown along with the comparison of the performance of the codes. Finally, conclusions will be drawn in Sec. 4.

2. Comparison of theoretical approaches to linear response calculations 2.1. Dyson-like equation

The dielectric function in eq. (1) is determined by the macroscopic density response function (or susceptibility) χM [8]:

M(Q, ω)−1 = 1 + vG(Q)χM(Q, ω), (2)

where vG(Q) = 4πe2/|Q|2 is the Fourier transform of the Coulomb potential. χM is related to

the microscopic density response function χG,G(q, ω):

χM(Q, ω) = χG,G(q, ω), (3)

where Q = q + G, with G being a reciprocal lattice vector and q a wavevector in the first Brillouin zone. Within the traditional linear response approach of TDDFT, χ of the interacting many-body system is related to the density response function χ0 of the non-interacting Kohn-Sham (KS) system through a Dyson-like screening equation:

χ = χ0+ (v + fxc)χ. (4)

fxc is the exchange-correlation kernel and χ0 is given by

χ0_{G,G}0(q, ω) =
1
V
BZ
X
k
X
n,n0
fn,k− fn0_{,k+q}
~ω + ε0n,k− ε0n0_{,k+q}+ iη
hϕ0
n,k|e
−i(q+G)r_{|ϕ}0
n0_{,k+q}ihϕ0_{n}0_{,k+q}|ei(q+G)r|ϕ0_{n,k}i,
(5)
where ϕ0_{n,k}, ε0_{n,k}, fn,k are respectively the unperturbed single-particle wavefunctions, their

eigenvalues and occupation numbers, V is the volume of the unit-cell and n, n0 are indices that span all of the occupied and unoccupied bands. The accurate calculation of χ in a wide frequency range using eq. (4) and (5) will require a separate calculation for each value of the frequency and knowledge of all of the empty states up to the requested energy, which makes this task cumbersome.

2.2. Sternheimer equations

On the other hand, the density response-function can be defined through the first-order correction to the density n(r, t) = n0(r) + n0(r, t) of the system under a weak external perturbation Vext(r, t) = Vext0 (r) + V0ext(r, t):

n0(r, t) = Z ∞ −∞ dt0 Z dr0χ(r, r0, t − t0)V0ext(r0, t0). (6)

In the case of EEL spectroscopy, the external perturbation is V0ext(r0, t0) ∼ ei(q·r−ωt). One

can perform a direct calculation of the χ using density functional perturbation theory (DFPT)
techniques without explicit calculation of empty states [9] and without solving the Dyson-like
equation (4). In this framework a system under external perturbation can be described by the
TDDFPT KS equation:
i~∂ϕn,k(r, t)
∂t = ˆH
KS_{(r, t)ϕ}
n,k(r, t), (7)
where ϕn,k(r, t) = ϕ0n,k(r) + ϕ
0

n,k(r, t) is the KS wavefunction decomposed into the unperturbed

KS wave and its first-order variation. ˆHKS_{(r, t) = ˆ}_{H}0_{(r) + V}0_{(r, t) is the KS Hamiltonian which}

consists in the static unperturbed Hamiltonian ˆH0(r) and of the (linearized) perturbation part
V0(r, t). This equation and its complex-conjugate can be linearized and, taking into account
only the first-order response, yield the so-called Sternheimer equation [9] which, in the frequency
domain, reads:
( ˆH0− ε0_{n,k}_{− ~ω)ϕ}0_{n,k}(r, ω) + ˆPcV
0
Hxc(r, ω)ϕ0n,k(r) = − ˆPcV
0
ext(r, ω)ϕ0n,k(r), (8)
( ˆH0− ε0_{n,−k}_{+ ~ω)ϕ}0_{n,−k}∗ (r, −ω) + ˆPcV
0_{∗}
Hxc(r, −ω)ϕ0n,k(r) = − ˆPcV
0_{∗}
ext(r, −ω)ϕ0n,k(r), (9)

where ˆPc is a projector on empty states and the first order correction to the density n0(r, t)

reads:
n0(r, t) =
BZ
X
k
X
n
ϕ0∗_{n,k}(r)hϕ0_{n,−k}∗ (r, −ω) + ϕ0_{n,k}(r, ω)i (10)
where n now only spans the occupied bands. For metals, partially occupied bands should be
accounted for using the smearing approach [10, 11]. However, for the sake of simplicity it is
ommited in the present work, and only the insulating case is considered. This set of equations
can be solved self-consistently for each value of ω, allowing us to obtain the susceptibility χ of
the system.

2.3. The Liouville-Lanczos equation

Equivalently, instead of eq. (7), one can use the quantum Liouville equation [12, 13, 14]: i~d ˆρ(t)

dt =

h ˆ_{H}_{KS}_{(t), ˆ}_{ρ(t)}i

, (11)

where ˆρ(t) is the reduced one-electron KS density-matrix whose kernel reads:

ρ(r, r0, t) =Xϕv(r, t)ϕ∗v(r0, t), (12)

and n(r, t) = ρ(r, r, t). Equation (11) can be linearized in the same manner as eq. (7), leading to the linearized Liouvillian equation:

(~ω − ˆL) · ˆρ¯0(ω) =h ˜V_{ext}0 (ω), ˆρ0
i

4

The action of the Liouvillian superoperator ˆL onto ˆρ is defined as: ˆ

L · ˆρ0=h ˆH0, ˆρ0i+V0

Hxc[ ˆρ0], ˆρ0 . (14)

Equation (13) can be solved using the Lanczos recursive scheme for all of the frequencies at once, resulting in the susceptibility χ.

2.4. Comparison of the methods

Each of three methods briefly described in Sec. 2.1 to 2.3 allows us to perform a first-principle calculation of the linear density response function χ(q, ω) and, thus, to obtain the dielectric and loss function of a given system, that can be directly compared to the experimental measurements

(see eq. (1)). Each method has advantages and drawbacks, the understanding of which is

necessary to choose the approach the most adapted to the target-problem.

Calculation of χ using a Dyson-like equation [15] is a powerful method that allows one to access and analyze individual electronic excitations in the material. However, this information comes for a relatively high cost: computation of χ0 in eq. (5) requires the computation of corresponding empty states, and computation of χ in eq. (4) involves multiplication and inversion of large matrices, making this calculations demanding in terms of central processing unit (CPU) time and random access memory (RAM).

On the contrary, usage of DFPT techniques [9] in the Sternheimer approach allows one to avoid the computation of the (numerous) empty states, by introducing the projector on the empty states ˆPcin eq. (8) and (9). This reduces the RAM and CPU time usage. Nevertheless,

the CPU time usage will remain high for the calculation over a wide frequency range, as the
self-consistent solution of eq. (8) and (9) should be repeated for each value of the desired frequency.
The Lanczos recursion algorithm used to solve the linearized Liouvillian equation (13) allows
us to avoid the explicit computation of the susceptibility for each frequency value, separating
the calculation into two steps. The first step of the Lanczos recursion is time consuming.
It is used to generate a tridiagonal matrix of coefficients which is used in the second step
(post-processing) to calculate the frequency-dependent susceptibility χ. This scheme allows
one to reduce CPU time usage significantly. However, there are two main drawbacks of the
Liouville-Lanczos approach: firstly, it is possible to perform calculations only in the case of
an adiabatic exchange and correlation functional V_{Hxc}0 in eq. (14). In the case where V_{Hxc}0
has an explicit frequency dependence, one will have to repeat the recursive procedure for each
desired value of the frequency, increasing the CPU time tremendously, therefore making this
procedure inefficient. Secondly, within both Liouville-Lanczos and Sternheimer approaches, it
is not possible to retrieve the information from which orbitals a specific peak in a spectrum
consists of, thus making an analysis for understanding the physical origins more demanding.
3. Comparison of the results and performance of two codes: turboEELS and
thermo pw

3.1. Computational details

Ground state properties have been calculated using the density functional theory (DFT) [16, 17] in the plane wave and pseudopotential method within the local density approximation [18] for bismuth and the generalized gradient approximation [19] for gold.

For bulk Bi, a 2-atom trigonal unit-cell was used, with a plane wave basis set limited with a cutoff energy of 60 Ry. A Monkhorst-Pack grid of 143 k-points has been used to sample the Brillouin zone [20]. For the calculation of EEL spectra, a small transferred momentum of q = 0.013˚A−1in the (111) trigonal direction was chosen. An imaginary frequency was introduced, so that ~ω in eq. (8) and (9) reads ~ω + iη, with η = 0.135eV . Indeed, the Sternheimer equations are solved with this broadening. At variance, in the Liouville-Lanczos method the broadening is

used only in the post-processing step, when the χ response function is built from the recursion coefficients. Calculations were performed using both scalar-relativistic - no spin-orbit coupling (SOC) and full-relativistic - with SOC normconserving pseudopotentials [21]. The number of iterations in the Lanczos recursion was 8000.

For bulk Au a 1-atom face-centered cubic unit-cell was used, with a plane wave basis set limited with a cutoff energy of 60 Ry. A Monkhorst-Pack grid of 323 k-points has been used to sample the Brillouin zone. For the calculation of EEL spectra, a small transferred momentum of q = 0.039˚A−1 was used and an imaginary frequency η = 0.135eV was added. Calculations were performed using scalar relativistic (without SOC) normconserving pseudopotential [22]. The number of iterations in the Lanczos recursion was 5000.

Convergence was carefully checked. In the thermo pw the procedure has an explicit

convergence threshold parameter on the variation of the density. This threshold was set to 10−12. In the Liouville-Lanczos approach, the recursion chain should be cut after a certain number of iterations, meaning that convergence should be verified manually by performing additional iterations.

Both Sternheimer (thermo pw code, unpublished [23]) and the Liouville-Lanczos (turboEELS code [14]) approaches are implemented in the Quantum ESPRESSO package for electronic structure calculations [24, 25]. Both codes support normconserving and ultrasolf

pseudopotentials. Several levels of MPI parallelization are implemented: a plane-wave

parallelization and a k-point parallelization. 3.2. Results

In figure 1, we report EEL spectra for bulk Bi obtained both with the thermo pw code, and with turboEELS : results are in perfect agreement with each other and with previous calculations [3], both with and without SOC. We point out that the TDDFPT calculations were performed with, as input, data coming from the same (DFT) ground state self-consistent calculation.

Figure 2 shows the comparison of the EEL spectra for bulk Au obtained by thermo pw and turboEELS codes.Obtained results are in agreement with previous ab initio calculations of the EELS for Au [26]. In the figure 2 one can see a severely damped plasmon peak around 2.5 eV and numerous interband transition at higher energies.

Figure 3 shows the relative difference between EEL spectra computed with the thermo pw and turboEELS codes. Beyond 2 eV the agreement is perfect and the two codes agree within 1%. Below 2 eV, the loss function is tending to 0 and the magnitude of the relative difference becomes higher as the loss function does not tend to 0 in the same way. Indeed, oscillations that are intrinsic to the Lanczos, approach are magnified in the difference at low energy. As in the case for Bi, agreement is perfect, that indicates that both codes are well-suited to handle either semimetallic or metallic materials.

6 0 0.5 1 1.5 2 2.5 0 5 10 15 20 25 Loss function E, eV turboEELS without SOC thermo_pw without SOC turboEELS with SOC thermo_pw with SOC

Figure 1: Bulk Bi. Loss function for a

transferred momentum q = 0.013˚A−1 in

the z-direction obtained using: turboEELS

code without (——) and with —— spin-orbit

coupling (SOC), and thermo pw code without (

## ◦

) and with (## ◦

) SOC.Loss function

E, eV Bulk

plasmon

turboEELS without SOC thermo_pw without SOC

0 0.2 0.4 0.6 0.8 1 1.2 1.4 0 10 20 30 40 50 60 Interband transitions

Figure 2: Bulk Au. Loss function for a

vanishing transferred momentum is the x-direction, calculated with the turboEELS code

(——) and thermo pw code (- - - -). Shaded

area marks the energy region where our

pseudopotential is less accurate and arrows indicate the position of bulk plasmon and the region on interband transitions.

Loss(turboEELS)-Loss(thermo_pw), % E, eV 2 -4 -3 -2 -1 0 1 2 3 4 0 10 20 30 40 50 60

Figure 3: Bulk Au. Relative difference between the loss functions computed for a vanishing transferred momentum is the x-direction, calculated with the turboEELS and thermo pw codes.

3.3. Performance

In figure 4, we show the comparison of the performance of both codes in terms of CPU time for bulk Bi without SOC. One can see that the turboEELS code is more efficient than the thermo pw code on a wide frequency range. We note that calculations in a low frequency region (0-10 eV) are considerably faster, by a factor of 2-3, than in the middle and high frequency region (10-30 eV).

0 0.5 1 1.5 2 2.5 0 5 10 15 20 25 1 2 3 4 5 6 7 8 9 10

Loss function Time, hours

E, eV turboEELS without SOC

thermo_pw without SOC turboEELS time (whole spectrum) thermo_pw time (5 frequencies)

Figure 4: Bulk Bi. Performance comparison of turboEELS and thermo pw codes without

spin-orbit coupling. Loss functions obtained with turboEELS (——) and thermo pw (

## ◦

) codesare shown (left-hand side abscissa). Time required for turboEELS (- - - -) to compute the whole spectrum and for thermo pw ( ) to compute the loss function for five frequencies in the corresponding frequency range is shown (right-hand side abscissa).

to obtain curves in fig. 2 and 4. In the last column of table 1, the number of frequency is given, showing on average how many frequencies can be calculated with thermo pw when consuming the same amount of CPU time needed for turboEELS to calculate the whole spectra. We point out that the ratio may however depend on the selected frequency range.

Performance comparison for the calculation with SOC is not shown in the present work. Taking SOC into account roughly increases the required CPU time by a factor of 4 for both codes, without influencing their relative performance.

Table 1: Performance comparison of the turboEELS and thermo pw codes for bulk Bi and Au.

System # of CPU cores # of frequencies (ω) Time (h) average # of ω for thermo pw to

match turboEELS CPU time

Bi turboEELS 72 any 10

Bi thermo pw 72 130 118 11

Au turboEELS 240 any 0.75

Au thermo pw 240 600 16 28

4. Conclusions

In this work we have done a comparison between results and performance of the codes and corresponding methods that allow us to calculate EEL spectra. It has been found that results obtained using the Sternheimer equation and the Liouville-Lanczos approach are in perfect agreement with each other for semiconducting (not shown), semimetallic and metallic samples.

8

However, as anticipated in Sec. 2.4, the performance of the turboEELS code is significantly better when the range of frequencies is wide. In principle it is possible to calculate EEL spectra on a 0-250 eV range at the same computational cost as on the 0-25 eV interval, although it might be necessary to include core electrons in the pseudopotential in order to describe high-energy excitations correctly. One can see that it is convenient to use the thermo pw code for a precise calculation of the susceptibility in a narrow frequency range.

Acknowledgement

Calculations have been performed with the Quantum ESPRESSO packages [25]. Support from the ANR-10-LABX-0039-PALM program (Femtonic project), from the DGA (France), from the program NEEDS-Mat´eriaux (France) and from the Chaire ´Energie of the ´Ecole Polytechnique is gratefully acknowledged. Computer time was granted by ´Ecole Polytechnique through the LLR-LSI project, by GENCI (Project No. 2210) and by PRACE (Project No. 2010PA3750). Andrea Dal Corso acknowledges support from the European Union H2020-EINFRA-2015-1 programme under grant agreement No. 676598 project “MaX - materials at the exascale”.

References

[1] Egerton R F 1996 Electron Energy-Loss Spectroscopy in the Electron Microscope 2nd ed (New York and London: Plenum)

[2] Botti S, Schindlmayr A, Sole R D and Reining L 2007 Rep. Prog. Phys. 70 357

[3] Timrov I, Markov M, Gorni T, Raynaud M, Motornyi O, Gebauer R, Baroni S and Vast N 2017 Phys. Rev. B 95 094301

[4] See in particular Ref. 9-14 and 28-48 of Ref. [3]

[5] Olevano V and Reining L 2001 Phys. Rev. Lett. 86 5962 [6] Runge E and Gross E 1984 Phys. Rev. Lett. 52 997 [7] Gross E K U and Kohn W 1985 Phys. Rev. Lett. 55 2850

[8] Car R, Tosatti E, Baroni S and Leelaprute S 1981 Phys. Rev. B 24 985

[9] Baroni S, de Gironcoli S, Corso A D and Giannozzi P 2001 Rev. Mod. Phys. 73 515 [10] de Gironcoli S 1995 Phys. Rev. B 51 6773

[11] Methfessel M and Paxton A 1989 Phys. Rev. B 40 3616

[12] Rocca D, Gebauer R, Saas Y and Baroni S 2008 J. Chem. Phys. 128 154105 [13] Timrov I, Vast N, Gebauer R and Baroni S 2014 Phys. Rev. B 88 064301

[14] Timrov I, Vast N, Gebauer R and Baroni S 2015 Computer Physics Communications 06/2015 dOI: 10.1016/j.cpc.2015.05.021

[15] Onida G, Reining L and Rubio A 2002 Rev. Mod. Phys. 74 601 [16] Hohenberg P and Kohn W 1964 Phys. Rev. 136 B864

[17] Kohn W and Sham L 1965 Phys. Rev. 140 A1133 [18] Perdew J P and Zunger A 1981 Phys. Rev. B 23 5048

[19] Perdew J, Burke K and Ernzerhof M 1996 Phys. Rev. Lett. 77 3865 [20] Monkhorst H and Pack J 1976 Phys. Rev. B 13 5188

[21] Markov M, Sjakste J, Fugallo G, Paulatto L, Lazzeri M, Mauri F and Vast N 2016 Phys. Rev. B 93 064301 [22] Pseudopotential was generated using parameters provided in http://bohr.inesc-mn.pt/~jlm/pseudo.html [23] Code can be obtained from http://people.sissa.it/~dalcorso/thermo_pw_dist.html

[24] Giannozzi P, Baroni S, Bonini N, Calandra M, Car R, Cavazzoni C, Ceresoli D, Chiarotti G, Cococcioni M, Dabo I, Dal Corso A, De Gironcoli S, Fabris S, Fratesi G, Gebauer R, Gerstmann U, Gougoussis C, Kokalj A, Lazzeri M, Martin-Samos L, Marzari N, Mauri F, Mazzarello R, Paolini S, Pasquarello A, Paulatto L, Sbraccia C, Scandolo S, Sclauzero G, Seitsonen A, Smogunov A, Umari P and Wentzcovitch R 2009 J. Phys.: Condens. Matter 21 395502

[25] Giannozzi P, Andreussi O, Brumme T, Bunau O, Nardelli M B, Calandra M, Car R, Cavazzoni C, Ceresoli D, Cococcioni M, Colonna N, Carnimeo I, Corso A D, de Gironcoli S, Delugas P, Ferretti R A D J A, Floris A, Fratesi G, Fugallo G, Gebauer R, Gerstmann U, Giustino F, Gorni T, Jia J, Kawamura M, Ko H Y, Kokalj A, K¨u¸c¨ukbenli E, Lazzeri M, Marsili M, Marzari N, Mauri F, Nguyen N L, Nguyen H V, de-la Roza A O, Paulatto L, Ponc´e S, Rocca D, Sabatini R, Santra B, Schlipf M, Seitsonen A P, Smogunov A, Timrov I, Thonhauser T, Umari P, Vast N, Wu X and Baroni S 2017 J. Phys.: Condens. Matter 29 465901 URL http://www.quantum-espresso.org